#------------------------------------------------------------------------------
#$Date: 2019-07-04 03:16:03 +0300 (Thu, 04 Jul 2019) $
#$Revision: 216715 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/55/19/1551951.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1551951
loop_
_publ_author_name
'Wang, Long-Fei'
'Zhuang, Wei-Man'
'Guo-Zhang, Huang'
'Chen, Yan-Cong'
'Qiu, Jiang-Zhen'
'Ni, Zhao-Ping'
'Tong, Ming-Liang'
_publ_section_title
;
 Spin-Crossover Modulation via Single-Crystal to Single-Crystal
 Photochemical [2+2] Reaction in Hofmann-Type Frameworks
;
_journal_name_full               'Chemical Science'
_journal_paper_doi               10.1039/C9SC02274K
_journal_year                    2019
_chemical_formula_moiety         '0.5(C60 H44 Ag4 Fe2 N12)'
_chemical_formula_sum            'C30 H22 Ag2 Fe N6'
_chemical_formula_weight         738.12
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_audit_creation_date             2018-07-23
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.18 svn.r3508 for OlexSys, GUI svn.r5497)
;
_audit_update_record
;
2019-02-18 deposited with the CCDC.    2019-07-03 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.2405(7)
_cell_length_b                   13.9694(9)
_cell_length_c                   16.0892(9)
_cell_measurement_reflns_used    9847
_cell_measurement_temperature    120
_cell_measurement_theta_max      27.46
_cell_measurement_theta_min      2.55
_cell_volume                     2751.1(3)
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      120
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0863
_diffrn_reflns_av_unetI/netI     0.0267
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.991
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            52006
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.991
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.628
_diffrn_reflns_theta_min         2.532
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.961
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.6545
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2014/5 (Bruker,2014/5) was used for absorption correction. wR2(int) was 0.0782 before and 0.0574 after correction. The Ratio of minimum to maximum transmission is 0.8778. The λ/2 correction factor is Not present.'
_exptl_crystal_colour            red
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    1.782
_exptl_crystal_description       block
_exptl_crystal_F_000             1456
_exptl_crystal_size_max          0.149
_exptl_crystal_size_mid          0.105
_exptl_crystal_size_min          0.055
_refine_diff_density_max         1.779
_refine_diff_density_min         -1.032
_refine_diff_density_rms         0.153
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.099
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     130
_refine_ls_number_reflns         3169
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.099
_refine_ls_R_factor_all          0.0591
_refine_ls_R_factor_gt           0.0482
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0127P)²+29.7219P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1002
_refine_ls_wR_factor_ref         0.1054
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2696
_reflns_number_total             3169
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9sc02274k2.cif
_cod_data_source_block           120k_CCDC1
_cod_database_code               1551951
_shelx_shelxl_version_number     2017/1
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.900
_shelx_estimated_absorpt_t_min   0.759
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(C6) = Uanis(C7)
Uanis(C9) = Uanis(C10) = Uanis(C11) = Uanis(C12) = Uanis(C13) = Uanis(C8)
3. Same fragment restrains
{N1, C5, C4, C3, C2, C1} sigma for 1-2: 0.02, 1-3: 0.04
as
{N1, C1, C2, C3, C4, C5}
4.a Ternary CH refined with riding coordinates:
 C6(H6), C7(H7)
4.b Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C4(H4), C5(H5), C9(H9), C10(H10), C11(H11), C12(H12), C13(H13)
4.c Fitted hexagon refined as free rotating group:
 C8(C9,C10,C11,C12,C13)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Ag1 Ag 0.23000(3) 1.04388(3) 0.26180(2) 0.02160(12) Uani 1 1 d . . .
Fe1 Fe 0.500000 1.000000 0.500000 0.00977(18) Uani 1 2 d S T P
N2 N 0.4021(3) 0.9701(3) 0.5912(2) 0.0145(8) Uani 1 1 d . . .
N3 N 0.3807(3) 1.0205(3) 0.4228(2) 0.0153(8) Uani 1 1 d . . .
C14 C 0.3528(4) 0.9578(4) 0.6508(3) 0.0194(10) Uani 1 1 d . . .
C15 C 0.3212(4) 1.0338(4) 0.3688(3) 0.0194(10) Uani 1 1 d . . .
N1 N 0.5070(3) 0.8614(3) 0.4685(2) 0.0147(8) Uani 1 1 d D . .
C1 C 0.4193(5) 0.8048(4) 0.4717(3) 0.0234(11) Uani 1 1 d D . .
H1 H 0.349244 0.833124 0.478414 0.028 Uiso 1 1 calc R . .
C2 C 0.4271(5) 0.7048(4) 0.4656(3) 0.0344(14) Uani 1 1 d D . .
H2 H 0.362864 0.666742 0.467908 0.041 Uiso 1 1 calc R . .
C3 C 0.5284(5) 0.6612(4) 0.4562(3) 0.0336(14) Uani 1 1 d D . .
C4 C 0.6163(5) 0.7205(4) 0.4449(3) 0.0323(13) Uani 1 1 d D . .
H4 H 0.685892 0.694413 0.431823 0.039 Uiso 1 1 calc R . .
C5 C 0.6033(4) 0.8185(4) 0.4527(3) 0.0226(11) Uani 1 1 d D . .
H5 H 0.666104 0.857882 0.446621 0.027 Uiso 1 1 calc R . .
C6 C 0.5504(6) 0.5544(4) 0.4663(4) 0.0351(10) Uani 1 1 d . . .
H6 H 0.621844 0.536088 0.440698 0.042 Uiso 1 1 calc R . .
C7 C 0.4592(6) 0.4852(4) 0.4400(4) 0.0351(10) Uani 1 1 d . . .
H7 H 0.391801 0.521243 0.424081 0.042 Uiso 1 1 calc R . .
C8 C 0.4877(4) 0.4096(3) 0.3730(2) 0.0463(7) Uani 1 1 d . . .
C9 C 0.5902(3) 0.3927(3) 0.3388(3) 0.0463(7) Uani 1 1 d G . .
H9 H 0.650614 0.431384 0.354545 0.056 Uiso 1 1 calc R . .
C10 C 0.6043(3) 0.3193(3) 0.2815(3) 0.0463(7) Uani 1 1 d G . .
H10 H 0.674307 0.307719 0.258115 0.056 Uiso 1 1 calc R . .
C11 C 0.5159(4) 0.2627(3) 0.2585(3) 0.0463(7) Uani 1 1 d G . .
H11 H 0.525512 0.212522 0.219309 0.056 Uiso 1 1 calc R . .
C12 C 0.4134(3) 0.2796(3) 0.2927(3) 0.0463(7) Uani 1 1 d G . .
H12 H 0.353022 0.240988 0.276934 0.056 Uiso 1 1 calc R . .
C13 C 0.3994(3) 0.3531(3) 0.3500(3) 0.0463(7) Uani 1 1 d G . .
H13 H 0.329327 0.364653 0.373365 0.056 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C14 Ag1 C15 174.3(2) 2_574 .
N2 Fe1 N2 180.0 5_676 .
N2 Fe1 N1 89.41(16) . 5_676
N2 Fe1 N1 89.41(16) 5_676 .
N2 Fe1 N1 90.59(16) . .
N2 Fe1 N1 90.59(16) 5_676 5_676
N3 Fe1 N2 87.06(16) . 5_676
N3 Fe1 N2 92.94(16) 5_676 5_676
N3 Fe1 N2 87.06(16) 5_676 .
N3 Fe1 N2 92.94(16) . .
N3 Fe1 N3 180.0 . 5_676
N3 Fe1 N1 90.72(16) . .
N3 Fe1 N1 89.28(16) . 5_676
N3 Fe1 N1 89.28(16) 5_676 .
N3 Fe1 N1 90.72(16) 5_676 5_676
N1 Fe1 N1 180.0 5_676 .
C14 N2 Fe1 172.1(4) . .
C15 N3 Fe1 170.4(4) . .
N2 C14 Ag1 171.6(4) . 2_575
N3 C15 Ag1 171.2(4) . .
C1 N1 Fe1 121.8(3) . .
C1 N1 C5 116.7(4) . .
C5 N1 Fe1 121.0(3) . .
N1 C1 H1 119.0 . .
N1 C1 C2 122.1(5) . .
C2 C1 H1 119.0 . .
C1 C2 H2 119.8 . .
C3 C2 C1 120.3(5) . .
C3 C2 H2 119.8 . .
C2 C3 C6 125.1(6) . .
C4 C3 C2 116.8(5) . .
C4 C3 C6 117.9(5) . .
C3 C4 H4 120.1 . .
C3 C4 C5 119.7(6) . .
C5 C4 H4 120.1 . .
N1 C5 C4 123.9(5) . .
N1 C5 H5 118.1 . .
C4 C5 H5 118.1 . .
C3 C6 H6 111.2 . .
C3 C6 C7 117.3(5) . .
C3 C6 C7 115.0(5) . 5_666
C7 C6 H6 111.2 . .
C7 C6 H6 111.2 5_666 .
C7 C6 C7 89.4(5) . 5_666
C6 C7 C6 90.6(5) . 5_666
C6 C7 H7 110.6 5_666 .
C6 C7 H7 110.6 . .
C6 C7 C8 117.2(5) . .
C8 C7 C6 115.7(5) . 5_666
C8 C7 H7 110.6 . .
C9 C8 C7 126.5(4) . .
C9 C8 C13 120.0 . .
C13 C8 C7 113.4(4) . .
C8 C9 H9 120.0 . .
C8 C9 C10 120.0 . .
C10 C9 H9 120.0 . .
C9 C10 H10 120.0 . .
C11 C10 C9 120.0 . .
C11 C10 H10 120.0 . .
C10 C11 H11 120.0 . .
C10 C11 C12 120.0 . .
C12 C11 H11 120.0 . .
C11 C12 H12 120.0 . .
C11 C12 C13 120.0 . .
C13 C12 H12 120.0 . .
C8 C13 H13 120.0 . .
C12 C13 C8 120.0 . .
C12 C13 H13 120.0 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ag1 C14 2.054(5) 2_574
Ag1 C15 2.056(5) .
Fe1 N2 1.940(4) .
Fe1 N2 1.940(4) 5_676
Fe1 N3 1.938(4) .
Fe1 N3 1.938(4) 5_676
Fe1 N1 2.004(4) .
Fe1 N1 2.004(4) 5_676
N2 C14 1.145(6) .
N3 C15 1.150(6) .
N1 C1 1.335(6) .
N1 C5 1.346(6) .
C1 H1 0.9500 .
C1 C2 1.404(7) .
C2 H2 0.9500 .
C2 C3 1.390(8) .
C3 C4 1.369(8) .
C3 C6 1.524(8) .
C4 H4 0.9500 .
C4 C5 1.385(7) .
C5 H5 0.9500 .
C6 H6 1.0000 .
C6 C7 1.611(8) 5_666
C6 C7 1.536(9) .
C7 H7 1.0000 .
C7 C8 1.547(7) .
C8 C9 1.3900 .
C8 C13 1.3900 .
C9 H9 0.9500 .
C9 C10 1.3900 .
C10 H10 0.9500 .
C10 C11 1.3900 .
C11 H11 0.9500 .
C11 C12 1.3900 .
C12 H12 0.9500 .
C12 C13 1.3900 .
C13 H13 0.9500 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Fe1 N1 C1 C2 -167.3(4) . .
Fe1 N1 C5 C4 168.3(4) . .
N1 C1 C2 C3 0.3(8) . .
C1 N1 C5 C4 -3.9(7) . .
C1 C2 C3 C4 -6.4(8) . .
C1 C2 C3 C6 167.1(5) . .
C2 C3 C4 C5 7.3(8) . .
C2 C3 C6 C7 -69.6(8) . 5_666
C2 C3 C6 C7 33.5(8) . .
C3 C4 C5 N1 -2.3(8) . .
C3 C6 C7 C6 -118.0(6) . 5_666
C3 C6 C7 C8 122.4(6) . .
C4 C3 C6 C7 -153.0(6) . .
C4 C3 C6 C7 103.8(7) . 5_666
C5 N1 C1 C2 4.8(7) . .
C6 C3 C4 C5 -166.7(5) . .
C6 C7 C8 C9 5.6(7) . .
C6 C7 C8 C9 -99.5(6) 5_666 .
C6 C7 C8 C13 -177.0(4) . .
C6 C7 C8 C13 77.8(6) 5_666 .
C7 C6 C7 C6 0.000(1) 5_666 5_666
C7 C6 C7 C8 -119.6(6) 5_666 .
C7 C8 C9 C10 177.2(5) . .
C7 C8 C13 C12 -177.5(4) . .
C8 C9 C10 C11 0.0 . .
C9 C8 C13 C12 0.0 . .
C9 C10 C11 C12 0.0 . .
C10 C11 C12 C13 0.0 . .
C11 C12 C13 C8 0.0 . .
C13 C8 C9 C10 0.0 . .
